### Standard Test Method for

### Standard Test Method for

### Determining Residual Stresses by the Hole-Drilling

### Determining Residual Stresses by the Hole-Drilling

### Strain-Gage Method

### Gage Method

11This standard is issued under the ﬁxed designation E 837; the number immediately following the designation indicates the year of

This standard is issued under the ﬁxed designation E 837; the number immediately following the designation indicates the year of

original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A

original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A

supers

superscript epsilon cript epsilon ((ee) indicates an editorial change since the last revision or reapproval.) indicates an editorial change since the last revision or reapproval.

INTRODUCTION INTRODUCTION

The hole-drilling strain-gage method determines residual stresses near the surface of an isotropic The hole-drilling strain-gage method determines residual stresses near the surface of an isotropic line

linear-ar-elaselastic materiatic material. l. It It involinvolves attachinves attaching g a a strastrain in rosetrosette te to to the surface, drillinthe surface, drilling g a a hole at hole at thethe geometric center of the rosette, and measuring the resulting relieved strains. The residual stresses geometric center of the rosette, and measuring the resulting relieved strains. The residual stresses within the removed material are then determined from the measured strains using a series of equations. within the removed material are then determined from the measured strains using a series of equations. 1.

1. ScoScopepe 1.1

1.1 Residual Stress DeterminationResidual Stress Determination:: 1.1.1

1.1.1 This test This test methmethod od specspeciﬁes a iﬁes a holehole-dril-drilling proceduling procedurere for determining residual stress proﬁles near the surface of an for determining residual stress proﬁles near the surface of an isotropic linearly elastic material. The test method is applicable isotropic linearly elastic material. The test method is applicable to residual stress proﬁle determinations where in-plane stress to residual stress proﬁle determinations where in-plane stress gradients are small. The stresses may remain approximately gradients are small. The stresses may remain approximately con

constastant nt witwith h depdepth th (“u(“unifniformorm” ” strstressesses) es) or or thethey y mamay y varvaryy signi

signiﬁcantﬁcantly ly with with deptdepth h (“non(“non-uni-uniformform” ” strestresses)sses). . The The mea- mea-sured workpiece may be “thin” with thickness much less than sured workpiece may be “thin” with thickness much less than the diameter of the drilled hole or “thick” with thickness much the diameter of the drilled hole or “thick” with thickness much gre

greateater r thathan n the the diadiametmeter er of of the the dridrillelled d holhole. e. OnlOnly y uniuniforformm stress measurements are speciﬁed for thin workpieces, while stress measurements are speciﬁed for thin workpieces, while both uniform and non-uniform stress measurements are both uniform and non-uniform stress measurements are speci-ﬁed for thick workpieces.

ﬁed for thick workpieces. 1.2

1.2 Stress Measurement RangeStress Measurement Range:: 1.2

1.2.1 .1 The The holhole-de-drilrillinling g metmethod hod can can ideidentintify fy in-in-plaplane ne re- re-sidua

sidual l strestresses near sses near the measured surfacthe measured surface e of of the workpiecthe workpiecee material. The method gives localized measurements that material. The method gives localized measurements that indi-cate the residual stresses within the boundaries of the drilled cate the residual stresses within the boundaries of the drilled hole.

hole. 1.2

1.2.2 This .2 This testest t metmethod hod appapplielies s in in cascases es whewhere re mamaterterialial behav

behavior is ior is linelinear-ar-elaselastic. In tic. In theortheoryy, , it it is is possipossible for ble for localocall yielding to occur due to the stress concentration around the yielding to occur due to the stress concentration around the drill

drilled ed hole, hole, for for isotisotropic (equi-biropic (equi-biaxiaaxial) l) resiresidual dual stresstresses ses ex- ex-ceeding 50 % of the yield stress, or for shear stresses in any ceeding 50 % of the yield stress, or for shear stresses in any dir

directection ion excexceedeeding ing 25 25 % % of of the the yieyield ld strstressess. . HowHoweveeverr, , inin practice it is found that satisfactory results can be achieved practice it is found that satisfactory results can be achieved providing the residual stresses do not exceed about 60 % of the providing the residual stresses do not exceed about 60 % of the material yield stress.

material yield stress.

1.3

1.3 Workpiece DamageWorkpiece Damage:: 1.3.1

1.3.1 The hole-driThe hole-drillinlling g methmethod od is often describeis often described d as “semi-as “semi-destructive” because the damage that it causes is localized and destructive” because the damage that it causes is localized and often does not signiﬁcantly affect the usefulness of the often does not signiﬁcantly affect the usefulness of the work-piece. In contrast, most other mechanical methods for piece. In contrast, most other mechanical methods for measur-ing residual stresses substantially destroy the workpiece. Since ing residual stresses substantially destroy the workpiece. Since hole drilling does cause some damage, this test method should hole drilling does cause some damage, this test method should be applied only in those cases either where the workpiece is be applied only in those cases either where the workpiece is expendable, or where the introduction of a small shallow hole expendable, or where the introduction of a small shallow hole will not signiﬁcantly affect the usefulness of the workpiece. will not signiﬁcantly affect the usefulness of the workpiece.

1.4

1.4 ThiThis s stastandandard does rd does not purponot purport rt to to addaddreress ss all all of of thethe sa

safefety ty coconcncerernsns, , if if ananyy, , asassosociciatated ed wiwith th its its ususe. e. It It is is ththee responsibility of the user of this standard to establish responsibility of the user of this standard to establish appro- priate

priate safety safety and and health health practices practices and and determine determine the the applica- applica-bility of regulatory limitations prior to use.

bility of regulatory limitations prior to use. 2.

2. Referenced Referenced DocumentsDocuments 2.1

2.1 ASTM Standards:ASTM Standards: 22

E 251

E 251 TTest est MethMethods ods for for PerfPerformaormance nce CharaCharactercteristiistics cs of of Metallic Bonded Resistance Strain Gages

Metallic Bonded Resistance Strain Gages 3. 3. TTerminologyerminology 3.1 3.1 SymbolsSymbols:: a a –

– _{= }_{= } _{calib}_{calib}_{rati}_{rati}_{on constant for isotropi}_{on constant for isotropi}_{c }_{c }_{stre}_{stre}_{sses}_{sses}
b

b –

– _{= }_{= } _{calib}_{calib}_{rati}_{rati}_{on constan}_{on constan}_{t for shear stresse}_{t for shear stresse}_{s}_{s}
a

a – –

jk

jk = = calibcalibratiration matrix for isotropon matrix for isotropic stresseic stressess

b b – –

jk

jk = = calibcalibratiration matrix for shear streon matrix for shear stressessses

D

D = = diamdiameter of the gage circle, see Taeter of the gage circle, see Table 1ble 1..

1

1_{Thi}_{Thi}_{s }_{s }_{test metho}_{test metho}_{d }_{d }_{is }_{is }_{und}_{und}_{er }_{er }_{the jurisd}_{the jurisd}_{icti}_{icti}_{on }_{on }_{of ASTM Commi}_{of ASTM Commi}_{ttee E28 }_{ttee E28 }_{on}_{on}
Mechani

Mechanical Testing and is cal Testing and is the direct the direct responresponsibility of Subcommittesibility of Subcommittee e E28.E28.13 on13 on

Residua

Residual l Stress Stress MeasuremMeasurement.ent.

Cur

Currenrent t editedition ion appapprovroved ed FebFeb. . 1, 1, 2002008. 8. PubPublishlished ed AprApril il 2002008. 8. OriOriginginallyally

approved in 1981. Last previous edition approved in 2001 as E 837 – 01

approved in 1981. Last previous edition approved in 2001 as E 837 – 01 ee11

.

.

2

2_{For referenced ASTM standards, visit the ASTM website, www.astm.org, or}_{For referenced ASTM standards, visit the ASTM website, www.astm.org, or}
contact ASTM Customer Service

contact ASTM Customer Service at at service@service@astm.oastm.org. Forrg. ForAnnual Book of ASTM Annual Book of ASTM

Standards

Standardsvolume information, refer to the standard’s Document Summary page onvolume information, refer to the standard’s Document Summary page on

the ASTM

the ASTM websitewebsite..

Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States.

D0 = diameter of the drilled hole

E = Young’s modulus

j = number of hole depth steps so far k = sequence number for hole depth steps

P = uniform isotropic (equi-biaxial) stress

P_{k } = isotropic stress within hole depth step k

p = uniform isotropic (equi-biaxial) strain

pk = isotropic strain after hole depth step k

Q = uniform 45° shear stress

Q_{k } = 45° shear stress within hole depth step k

q = uniform 45° shear strain

q_{k } = 45° shear strain after hole depth step k

T = uniform x-y shear stress

T k = x-y shear stress within hole depth step k

t = x-y shear strain

t _{k } = x-y shear strain after hole depth step k

T = (superscript) matrix transpose

a_{P} = regularization factor for P stresses

a_{Q} = regularization factor for Q stresses

a_{T } = regularization factor for T stresses

b = clockwise angle from the x-axis (gage 1) to the maximum principal stress direction

e = relieved strain for “uniform” stress case

e_{ j} = relieved strain measured after j hole depth steps
have been drilled

n = Poisson’s ratio

u = angle of strain gage from the x-axis

s_{max } = maximum (more tensile) principal stress

a_{min} = minimum (more compressive) principal stress

s_{ x } = uniform normal x-stress

(s_{ x })k = normal x-stress within hole depth step k

s_{ y} = uniform normal y-stress

(s_{ y})_{k } = normal y-stress within hole depth step k

t_{ xy} = uniform shear xy-stress

(t_{ xy})k = shear xy-stress within hole depth step k

4. Summary of Test Method 4.1 Workpiece:

4.1.1 A ﬂat uniform surface area away from edges and other irregularities is chosen as the test location within the workpiece of interest. Fig. 1 schematically shows the residual stresses acting at the test location at which a hole is to be drilled. These stresses are assumed to be uniform within the in-plane direc-tions x and y.

NOTE 1—For reasons of pictorial clarity in Fig. 1, the residual stresses

are shown as uniformly acting over the entire in-plane region around the test location. In actuality, it is not necessary for the residual stresses to be uniform over such a large region. The surface strains that will be relieved by drilling a hole depend only on the stresses that originally existed at the boundaries of the hole. The stresses beyond the hole boundary do not affect the relieved strains, even though the strains are measured beyond the hole boundary. Because of this, the hole-drilling method provides a very localized measurement of residual stresses.

4.1.2 Fig. 1(a) shows the case where the residual stresses in
the workpiece are uniform in the depth direction. The in-plane
stresses are s_{x}, s_{y} and t_{xy} throughout the thickness. Uniform
residual stress measurements can be made using this test
method with “thin” workpieces whose material thickness is
small compared with the hole and strain gage circle diameters,
and with “thick” workpieces whose material thickness is large
compared with the hole and strain gage circle diameters.

4.1.3 Fig. 1(b) shows the case where the residual stresses in
the workpiece vary in the depth direction. The calculation
method described in this test method represents the stress
proﬁle as a staircase shape, where the depth steps correspond to
the depth increments used during the hole-drilling
measure-ments. Within depth step k , the in-plane stresses are (s_{x})k , (sy)k

and (t_{xy})_{k }. Non-uniform residual stress measurements can be
made using this test method only with “thick” workpieces
whose material thickness is large compared with the hole and
strain gage circle diameters.

4.2 Strain Gage Rosette::

4.2.1 A strain gage rosette with three or more elements of the general type schematically illustrated in Fig. 2 is attached to the workpiece at the location under consideration.

4.3 Hole-Drilling:

4.3.1 A hole is drilled in a series of steps at the geometric center of the strain gage rosette.

4.3.2 The residual stresses in the material surrounding the drilled hole are partially relieved as the hole is drilled. The associated relieved strains are measured at a speciﬁed sequence of steps of hole depth using a suitable strain-recording instru-ment.

4.4 Residual Stress Calculation Method :

4.4.1 The residual stresses originally existing at the hole location are evaluated from the strains relieved by hole-drilling using mathematical relations based on linear elasticity theory

(a)

(b)

FIG. 1 Hole Geometry and Residual Stresses, (a) Uniform Stresses, (b) Non-uniform Stresses

(1-5)).3_{The relieved strains depend on the residual stresses that}

existed in the material originally within the hole.

4.4.2 For the uniform stress case shown in Fig. 1(a), the surface strain relief measured after hole-drilling is:

e 5 1_{ E }1 n a s x 1 s y

2 (1)

1_{ E }1b s x –_{2}s y cos 2u
1_{ E }1 bt xy sin 2u

4.4.3 The calibration constants a–and b–indicate the relieved strains due to unit stresses within the hole depth. They are dimensionless, almost material-independent constants. Slightly different values of these constants apply for a

through-thickness hole made in a thin workpiece and for a blind hole made in a thick workpiece. Numerical values of these calibra-tion constants have been determined from ﬁnite element calculations (4) for standard rosette patterns, and are tabulated in this test method.

4.4.4 For the non-uniform stress case shown in Fig. 1(b), the surface strain relief measured after completing hole depth step j depends on the residual stresses that existed in the material

originally contained in all the hole depth steps 1 # k # j:

e_{ j}5 1_{ E }1 n

_{(}

k 51
j
a_{ jk }~~s

_{ x }1 s

_{ y}! / 2!

_{k }(2) 1

_{ E }1

_{(}

k 51
j
b_{ jk }~~s

_{ x }–s

_{ y}! / 2!

_{k }cos 2u 1

_{ E }1

_{(}

k 51
j
b_{ jk }~t

_{ xy}!

_{k }sin 2u

4.4.5 The calibration constants a– jk and b

–

jk indicate the

relieved strains in a hole j steps deep, due to unit stresses within hole step k . Fig. 3 shows cross-sections of drilled holes for an example sequence where a hole is drilled in four depth steps. Within this sequence, calibration constant represents an intermediate stage where the hole has reached 3 steps deep, and has a unit stress acting within depth step 2. Numerical values of the calibration constants have been determined by ﬁnite element calculations (4) for standard rosette patterns, and are tabulated in this test method.

4.4.6 Measurement of the relieved strains after a series of
hole depth steps provides sufficient information to calculate the
stresses s_{x}, s_{y} and t_{xy} within each step. From these stresses,
the corresponding principal stresses s_{max} and s_{min} and their
orientationb can be found.

4.4.7 The relieved strains are mostly inﬂuenced by the near-surface residual stresses. Interior stresses have inﬂuences that diminish with their depth from the surface. Thus, hole-drilling measurements can evaluate only near-surface stresses. Deep interior stresses cannot be identiﬁed reliably, see Note 7.

3_{The boldface numbers in parentheses refer to the list of references at the end of }

this standard.

(a)

(b)

FIG. 2 Schematic Geometry of a Typical Three-Element Clockwise (CW) Hole-Drilling Rosette, (a) Rosette Layout, (b)

Detail of a Strain Gage

4.4.8 In theory, it is possible for local yielding to occur due to the stress concentration around the drilled hole. Such yielding can occur with isotropic residual stresses exceeding 50 % of the yield stress, and for shear stresses exceeding 25 % of the yield stress. However, in practice it is found that satisfactory results can be achieved providing the residual stresses do not exceed about 60 % of the material yield stress (6).

5. Signiﬁcance and Use 5.1 Summary:

5.1.1 Residual stresses are present in almost all materials. They may be created during the manufacture or during the life of the material. If not recognized and accounted for in the design process, residual stresses can be a major factor in the failure of a material, particularly one subjected to alternating service loads or corrosive environments. Residual stress may also be beneﬁcial, for example, the compressive stresses produced by shot peening. The hole-drilling strain-gage tech-nique is a practical method for determining residual stresses. 6. Workpiece Preparation

6.1 Requirements:

6.1.1 For a “thin” workpiece, where a through-hole is to be used, the workpiece thickness should not exceed 0.4D for a type A or B rosette, or 0.48D for a type C rosette (see Fig. 4). 6.1.2 For a “thick” workpiece, where a hole depth less than the workpiece thickness is to be used, the workpiece thickness should be at least 1.2D for a type A or B rosette, or 1.44D for a type C rosette (see Fig. 4).

6.1.3 A smooth surface is usually necessary for strain gage application. However, abrading or grinding that could appre-ciably alter the surface stresses must be avoided. Chemical etching could be used, thus avoiding the need for mechanical abrasion.

6.1.4 The surface preparation prior to bonding the strain gages shall conform to the recommendations of the manufac-turer of the adhesive used to attach the strain gages. A thorough cleaning and degreasing is required. In general, surface prepa-ration should be restricted to those methods that have been demonstrated to induce no signiﬁcant residual surface stresses. This is particularly important for workpieces that contain sharp near-surface stress gradients.

7. Strain Gages and Instrumentation 7.1 Rosette Geometry:

7.1.1 A rosette comprising three single or pairs of strain gage grids shall be used. The numbering scheme for the strain gages follows a clockwise (CW) convention (7).

NOTE 2—The gage numbering scheme used for the rosette illustrated in

Fig. 2 differs from the counter-clockwise (CCW) convention often used for general-purpose strain gage rosettes and for some other types of residual stress rosette. If a strain gage rosette with CCW gage numbering is used, the residual stress calculation procedure described in this test method still applies. The only changes are that the numbering of gages 1 and 3 are interchanged and that the anglebdeﬁning the direction of the most tensile principal stresssmax is reversed and is measured

counter-clockwise from the new gage 1.

NOTE 3—It is recommended that the gages be calibrated in accordance

with Test Methods E 251.

7.1.2 The gages shall be arranged in a circular pattern, equidistant from the center of the rosette.

7.1.3 The gage axes shall be oriented in each of three directions, (1) a reference direction, (2) 45° or 135° to the reference direction, and (3) perpendicular to the reference direction. Direction (2) bisects directions (1) and (3), as shown in Fig. 2.

7.1.4 The measurement direction of gage 1 in Fig. 1 is identiﬁed as the x-axis. The y-axis is 90° counterclockwise of the x-axis.

7.1.5 The center of the gage circle shall be clearly identiﬁ-able.

7.2 Standardized Rosettes:

7.2.1 Several different standardized rosettes are available to meet a wide range of residual stress measurement needs. The use of standardized rosette designs greatly simpliﬁes the calculation of the residual stresses. Fig. 4 shows three different rosette types and Table 1 lists their dimensions.

7.2.2 The type A rosette shown in Fig. 4 was ﬁrst introduced by Rendler and Vigness (5). This pattern is available in several different sizes, and is recommended for general-purpose use.

NOTE 4—Choice of rosette size is a primary decision. Larger rosettes

tend to give more stable strain measurements because of their greater capacity to dissipate heat. They are also able to identify residual stresses to greater depths. Conversely, smaller rosettes can ﬁt smaller workpieces, require smaller drilled holes, and give more localized measurements.

7.2.3 The type B rosette shown in Fig. 4 has all strain gage grids located on one side. It is useful where measurements need to be made near an obstacle.

7.2.4 The type C rosette shown in Fig. 4 is a special-purpose pattern with three pairs of opposite strain gage grids that are to be connected as three half-bridges. It is useful where large strain sensitivity and high thermal stability are required (8).

7.3 Installation and Use:

7.3.1 The strain gage rosette should be attached to the workpiece surface such that its center is at least 1.5D from the nearest edge, or the boundary of another material should the workpiece be comprised of more than one material.

7.3.2 When using a type B rosette adjacent to an obstacle, the center of the rosette should be at least 0.5D from the obstacle, with the set of strain gages diametrically opposite to the obstacle.

7.3.3 The application of the strain gage (bonding, wiring, protective coating) should closely follow the manufacturer’s recommendations, and shall ensure the protection of the strain gage grid during the drilling operation.

7.3.4 The strain gages should remain permanently con-nected and the stability of the installation shall be veriﬁed. A resistance to ground of at least 20 000 MV is preferable.

7.3.5 Checks should be made to validate the integrity of the gage installation. If possible, a small mechanical load should be applied to the workpiece to induce some modest strains. The observed strains should return to zero when the load is removed. In addition, a visual inspection of the rosette instal-lation should be made to check for possible areas that are not well bonded. If incomplete bonding is observed, the rosette must be removed and replaced.

7.4 Instrumentation:

7.4.1 The instrumentation for recording of strains shall have a strain resolution of 61310-6, and stability and repeatability of the measurement shall be at least 61310-6. The lead wires from each gage should be as short as practicable and a three-wire temperature-compensating circuit (9) should be used with rosette types A and B. Half-bridge circuits should be

used with rosette type C, the resulting outputs of which are
designatede_{1}, e_{2}, and e_{3}.

8. Procedure

8.1 Suggested Preparatory Reading:

8.1.1 References (10) and (11) provide substantial practical guidance about how to make high-quality hole-drilling residual stress measurements. These publications are excellent prepa-ratory reading, particularly for practitioners who infrequently make hole-drilling measurements.

8.2 Drilling Equipment and Use:

8.2.1 A device that is equipped to drill a hole in the test workpiece in a controlled manner is required. The device must be able to drill a hole aligned concentric with the strain gage circle to within either 60.004D. It shall also be able to control the depth of the hole to within either 60.004D. Fig. 5 illustrates a typical hole-drilling apparatus.

8.2.2 Several drilling techniques have been investigated and reported to be suitable for the hole drilling method. The most common drilling technique suitable for all but the hardest materials involves the use of carbide burs or endmills driven by a high-speed air turbine or electric motor rotating at 50 000 to 400 000 rpm (13). Low-speed drilling using a drill-press or power hand-drill is discouraged because the technique has the tendency to create machining-induced residual stresses at the hole boundary (14).

TABLE 1 Rosette DimensionsA

Rosette Type D GLB _{GW}B _{R}
1B R2B
Type A
Conceptual D 0.309D 0.309D 0.3455D 0.6545D
1_{ ⁄ }
32in. nominal 0.101 0.031 0.031 0.035 0.066
(2.57) (0.79) (0.79) (0.89) (1.68)
1_{ ⁄ }_{16}_{in. nominal } _{0.202 } _{0.062 } _{0.062 } _{0.070 } _{0.132}
(5.13) (1.59) (1.59) (1.77) (3.36)
1_{ ⁄ }_{8}_{in. nominal } _{0.404 } _{0.125 } _{0.125 } _{0.140 } _{0.264}
(10.26) (3.18) (3.18) (3.54) (6.72)
Type B
Conceptual D 0.309D 0.223D 0.3455D 0.6545D
1_{ ⁄ }_{16}_{in. nominal } _{0.202 } _{0.062 } _{0.045 } _{0.070 } _{0.132}
(5.13) (1.59) (1.14) (1.77) (3.36)
Type C
Conceptual D 0.176D 30°
sector
0.412D 0.588D
1_{ ⁄ }_{16}_{in. nominal } _{0.170 } _{0.030 } _{30° } _{0.070 } _{0.100}
(4.32) (0.76) (30°) (1.78) (2.54)

A_{Dimensions are in inches (mm).}

B _{Rosette dimensions are deﬁned in Fig. 2.}

FIG. 5 A Typical Hole-Drilling Apparatus, (a) Optical Device for Centering the Tool Holder, (b) Hole-Drilling Tool

8.2.3 For very hard materials, abrasive jet machining can also be useful. This drilling method involves directing a high-velocity stream of air containing ﬁne abrasive particles through a small-diameter nozzle against the workpiece (5, 14). Abrasive jet machining can be less suitable for softer materials (7). It should not be used for non-uniform stress measurements because the hole geometry and depth cannot be controlled sufficiently tightly.

8.2.4 When using burs or endmills, carbide “inverted cone” dental burs or small carbide endmills can be suitable as cutting tools. Commercially available cutters are designed for a wide range of applications, and not all types may be suited for hole drilling residual stress measurements. Thus, a veriﬁcation of drilling technique and choice of cutter should be done when no prior experience is available. Veriﬁcation could consist of applying a strain gage rosette to a stress-free workpiece of the same nominal test material produced by the annealing heat treatment method (1, 5, 14, 15), and then drilling a hole. If the drilling technique and cutter are satisfactory, the strains pro-duced by the drilling will be small, typically within 68 µ e.

8.2.5 If the drilling technique veriﬁcation shows signiﬁcant strains induced by the drilling process, or if the test material is known to be difficult to machine, it may be helpful to lubricate the drilling cutter with a suitable lubricating ﬂuid. The ﬂuid used must be electrically non-conductive. Aqueous or other electrically conductive lubricants must not be used because they may penetrate the strain gage electrical connections and distort the strain readings.

8.2.6 The radial clearance angles of the cutting edges on the end face of the cutting tool should not exceed 1°. This requirement avoids ambiguities in hole depth identiﬁcation by ensuring that the depth is uniform within 1 % of the tool diameter.

8.2.7 “Inverted cone” cutters have their maximum diameter at their end face, tapering slightly towards the shank. The tapered geometry provides clearance for the cylindrical cutting edges as the tool cuts the hole. This feature is desirable because it minimizes tool rubbing on the side surface of the hole and possible localized residual stress creation. To avoid ambiguities in hole diameter identiﬁcation, the taper angle should not exceed 5° on each side.

8.2.8 Drilling may be done by plunging, where the cutter is advanced axially. Alternatively, an orbiting technique (16) may be used, where the rotation axis of the cutter is deliberately offset from the hole axis. The cutter is advanced axially, and is then orbited so that the offset traces a circular path and the cutter creates a hole larger than its diameter. The direct plunge method has the advantage of simplicity. The orbiting method has the advantages of hole diameter adjustment through choice of offset, use of the cylindrical cutting edges as well as those on the end surface, and clearer chip ﬂow.

8.2.9 Table 2 indicates the target hole diameter ranges appropriate for the various rosette types. Different ranges apply to uniform and non-uniform stress measurements.

8.2.10 The size of the measured strains increases approxi-mately proportionally with the square of the hole diameter. Thus, holes at the larger end of the range are preferred. If using the plunging method, the cutter diameter should equal the target diameter. If using the orbiting method, the cutter diameter should be 60 to 90 % of the target diameter, with an offset chosen to achieve a hole with the target diameter.

8.2.11 All drilling should be done under constant tempera-ture conditions. After each drilling step, the cutter should be stopped to allow time for stabilization of any temperature ﬂuctuations caused by the drilling process and air turbine

TABLE 2 Recommended Workpiece Thicknesses, Hole Diameters and Depth StepsA

Rosette Type D Max. thickness of a “Thin” workpiece Min. thickness of a “Thick” workpiece

Uniform Stresses Non-Uniform Stresses Min. hole diameter Max. hole diameter Practical depth stepsB Min. hole diameter Max. hole diameter Practical depth stepsB Type A

Conceptual D 0.4 D 1.2 D 0.6 Max D0 Max D0 0.05 D Min D0 Max D0 0.01 D

1_{ ⁄ }_{32}_{in. nominal } _{0.101 } _{0.040 } _{0.121 } _{0.024 } _{0.040 } _{0.005 } _{0.037 } _{0.040 } _{0.001}
(2.57) (1.03) (3.08) (0.61) (1.01) (0.25) (0.93) (1.00) (0.025)
1_{ ⁄ }_{16}_{in. nominal } _{0.202 } _{0.081 } _{0.242 } _{0.060 } _{0.100 } _{0.010 } _{0.075 } _{0.085 } _{0.002}
(5.13) (2.06) (6.17) (1.52) (2.54) (0.25) (1.88) (2.12) (0.05)
1_{ ⁄ }_{8}_{in. nominal } _{0.404 } _{0.162 } _{0.485 } _{0.132 } _{0.220 } _{0.020 } _{0.150 } _{0.170 } _{0.004}
(10.26) (4.11) (12.34) (3.35) (5.59) (0.50) (3.75) (4.25) (0.10)
Type B

Conceptual D 0.4 D 1.2 D 0.6 Max D0 Max D0 0.05 D Min D0 Max D0 0.01D

1_{ ⁄ }

16in. nominal 0.202 0.081 0.242 0.060 0.100 0.010 0.075 0.085 0.002

(5.13) (2.06) (6.17) (1.52) (2.54) (0.25) (1.88) (2.12) (0.05) Type C

Conceptual D 0.48 D 1.44 D 0.6 Max D0 Max D0 0.0575 D Min D0 Max D0 0.0115 D

1_{ ⁄ }_{16}_{in. nominal } _{0.170 } _{0.082 } _{0.245 } _{0.060 } _{0.100 } _{0.010 } _{0.075 } _{0.085 } _{0.002}

(4.32) (2.07) (6.22) (1.52) (2.54) (0.25) (1.88) (2.12) (0.05)

A_{Dimensions are in inches (mm).}
B _{See Note 6.}

exhaust. It is not essential to retract the cutter. Strain readings should attain their ﬁnal values for at least ﬁve seconds before being accepted.

8.2.12 Use the drilling procedure described in 8.3 when evaluating uniform stresses in a “thin” workpiece, in 8.4 for uniform stresses in a “thick” workpiece, and in 8.5 for non-uniform stresses in a “thick” workpiece.

8.3 Drilling Procedure for a “Thin” Workpiece with Uni- form Stresses:

8.3.1 For a “thin” workpiece, as deﬁned in 6.1.1, obtain an initial reading from each gage before starting the drilling operation.

8.3.2 Start the cutter and slowly advance it until it cuts
through the entire thickness of the workpiece. If using the
orbiting technique, also orbit the cutter. Stop and retract the
cutter. Then measure one set of strain readings e_{1}, e_{2} and e_{3}.
8.3.3 Measure the hole diameter and conﬁrm that it lies
within the target range speciﬁed in Table 2.

8.3.4 Check the hole concentricity and conﬁrm that it lies within the tolerance speciﬁed in 8.2.1.

8.3.5 Compute uniform residual stresses as described in 9.1. 8.4 Drilling Procedure for a “Thick” Workpiece with Uni- form Stresses:

8.4.1 For a “thick” workpiece, as deﬁned in 6.1.2, obtain an initial reading from each gage before starting the drilling operation. Start the cutter and slowly advance it until it cuts through the rosette backing material and lightly scratches the workpiece surface. This point corresponds to “zero” cutter depth.

NOTE 5—Some practitioners use a technique that identiﬁes the “zero”

point by the completion of an electrical connection between the cutter and the workpiece.

8.4.2 Stop the cutter after reaching the “zero” point and conﬁrm that all strain gage readings have not signiﬁcantly changed. Use the new readings as the zero points for the subsequent strain measurements.

8.4.3 Start the cutter and advance it by 0.05 D for a type A
or B rosette, or 0.06D for a type C rosette. If using the orbiting
technique, also orbit the cutter. Stop the cutter and record the
readings from each strain gage, e_{1}, e_{2} and e_{3}. Other similar
depth increments are acceptable; however, they are less
con-venient for calculations because they will require additional
interpolations of the calibration constants listed in Table 3.

NOTE 6—For practical measurements, the required cutter advance can

be approximated as 0.005 in. (0.125 mm) for a 1_{ ⁄ }_{32} _{in. Type A rosette,}

0.010 in. (0.25 mm) for a1_{ ⁄ }_{16}_{in. Type A, B or C rosette, or 0.020 in. (0.5}

mm) for a 1_{ ⁄ }_{8} _{in. Type A rosette (see Table 2). The associated small}

deviations from the speciﬁed 0.05D or 0.06D values do not signiﬁcantly affect the calculated residual stress results.

8.4.4 Repeat the stepwise advance in hole depth followed by strain measurements to a total of 8 equal hole depth steps, reaching a ﬁnal hole depth approximately equal to 0.4D for a type A or B rosette, or 0.48D for a type C rosette.

NOTE 7—A ﬁnal depth of 0.4D or 0.48D is used because the measured

strains continue to increase until this depth is reached. However, the measured strains mostly depend on the near-surface stresses, with sensi-tivity diminishing to near zero for stresses beyond 0.2D depth with Type A and B rosettes, or 0.3D depth with a Type C rosette. Thus, hole-drilling

measurements indicate a weighted average of the residual stresses within the near-surface layer, 0.2D or 0.3D deep from the measured surface.

8.4.5 Measure the hole diameter and conﬁrm that it lies within the target range speciﬁed in Table 2.

8.4.6 Check the hole concentricity and conﬁrm that it lies within the tolerance speciﬁed in 8.2.1.

8.4.7 Compute uniform residual stresses as described in 9.2. 8.5 Drilling Procedure for a “Thick” Workpiece with Non-Uniform Stresses:

8.5.1 Obtain zero readings from each gage before starting the drilling operation. Start the cutter and carefully advance it until it cuts through the rosette backing material and lightly scratches the workpiece surface. This point corresponds to “zero” cutter depth (see Note 5).

8.5.2 Stop the cutter after reaching the “zero” point and conﬁrm that all strain gage readings have not signiﬁcantly changed. Use the new readings as the zero points for the subsequent strain measurements.

8.5.3 Start the cutter and advance it by 0.001 in. (0.025 mm)
for a 1_{ ⁄ }_{32} _{in. Type A Rosette, 0.002 in. (0.05 mm) for a} 1_{ ⁄ }_{16} _{in.}

Type A, B or C Rosette, or 0.004 in. (0.10 mm) for a1_{ ⁄ }_{8}_{in. Type}

A Rosette. Stop the cutter and record the readings from each strain gage.

8.5.4 When working with a Type A or B Rosette, repeat the stepwise advance in hole depth followed by strain measure-ments to a total of 20 equal hole depth steps.

8.5.5 When working with a Type C Rosette, repeat the stepwise advance in hole depth followed by strain measure-ments to a total of 25 equal hole depth steps.

8.5.6 Measure the hole diameter and conﬁrm that it lies within the target range speciﬁed in Table 2.

8.5.7 Check the hole concentricity and conﬁrm that it lies within the tolerance speciﬁed in 8.2.1.

8.5.8 Compute non-uniform residual stresses as described in Section 10.

9. Computation of Uniform Stresses 9.1 “Thin” Workpiece:

9.1.1 Compute the following combination strains for the
measured strains e_{1}, e_{2}, e_{3}:

p5~e31 e1! / 2 (3)

q5~e3–e1! / 2 (4)

t 5~e31 e1– 2e2! / 2 (5)

9.1.2 Use Table 3 to determine the numerical values of the calibration constants a– and b– corresponding to the hole diameter and type of rosette used.

9.1.3 Compute the three combination stresses P, Q and T
corresponding to the three combination strains p, q and t using
(4):
P 5 s y1 s_{2} x 5 – E p
a~11 n! (6)
Q5 s y–_{2}s x 5 – E q
b (7)
T 5 t_{ xy} 5 – E t
b (8)

where:

P = isotropic (equi-biaxial) stress, Q = 45° shear stress, and

T = xy shear stress.

9.1.4 Compute the in-plane Cartesian stressess_{x},s_{y}andt_{xy}

using:

s x 5 P–Q (9)

s_{ y}5 P1Q (10)

t_{ xy} 5 T (11)

9.1.5 Compute the principal stresses s_{max} ands_{min}using:

s_{max },s_{min} 5 P 6

### =

Q21T 2 (12)9.1.6 The more tensile (or less compressive) principal stress

s_{max} is located at an angle b measured clockwise from the
direction of gage 1 in Fig. 2. Similarly, the less tensile (or more
compressive) principal stress s_{min} is located at an angle b

measured clockwise from the direction of gage 3. 9.1.7 Compute the angleb using:

b 5 1_{2} arctan

## S

_{–}–

_{Q}T

## D

(13)9.1.8 Calculation of the angle b using the common one-argument arctan function, such as is found on an ordinary calculator, can give an ambiguity of 690°. The correct angle can be found by using the two-argument arctan function (function atan2 in some computer languages), where the signs of the numerator and denominator are each taken into account. Alternatively, the result from the one-argument calculation can be adjusted by adding or subtracting 90° as necessary to place

b within the appropriate range deﬁned in Table 4.

9.1.9 A positive value of b, sayb= 30°, indicates that s_{max}

lies 30° clockwise of the direction of gage 1. A negative value
of b, say b = –30°, indicates that s_{max} lies 30°
counter-clockwise of the direction of gage 1. In general, the direction

TABLE 3 Numerical Values of Coefficients a¯ and b¯ for Uniform Stress Evaluations

Rosette A a¯ b¯

Blind hole Hole Diameter, D0 /D Hole Diameter, D0 /D

Depth/D 0.30 0.35 0.40 0.45 0.50 0.30 0.35 0.40 0.45 0.50 0.00 .000 .000 .000 .000 .000 .000 .000 .000 .000 .000 0.05 .027 .037 .049 .063 .080 .051 .069 .090 .113 .140 0.10 .059 .081 .108 .138 .176 .118 .159 .206 .255 .317 0.15 .085 .115 .151 .192 .238 .180 .239 .305 .375 .453 0.20 .101 .137 .177 .223 .273 .227 .299 .377 .459 .545 0.25 .110 .147 .190 .238 .288 .259 .339 .425 .513 .603 0.30 .113 .151 .195 .243 .293 .279 .364 .454 .546 .638 0.35 .113 .151 .195 .242 .292 .292 .379 .472 .566 .657 0.40 .111 .149 .192 .239 .289 .297 .387 .482 .576 .668 Through Hole .090 .122 .160 .203 .249 .288 .377 .470 .562 .651 Rosette B a¯ b¯

Blind Hole Hole Diameter, D0 /D Hole Diameter, D0 /D

Depth/D 0.30 0.35 0.40 0.45 0.50 0.30 0.35 0.40 0.45 0.50 0.00 .000 .000 .000 .000 .000 .000 .000 .000 .000 .000 0.05 .029 .039 .053 .068 .086 .058 .078 .102 .127 .157 0.10 .063 .087 .116 .148 .189 .134 .179 .231 .286 .355 0.15 .090 .123 .162 .205 .254 .203 .269 .343 .419 .504 0.20 .107 .145 .189 .236 .289 .256 .336 .423 .511 .605 0.25 .116 .156 .202 .251 .305 .292 .381 .476 .571 .668 0.30 .120 .160 .206 .256 .309 .315 .410 .509 .609 .707 0.35 .120 .160 .206 .256 .308 .330 .427 .529 .631 .730 0.40 .118 .158 .203 .253 .305 .337 .437 .541 .644 .743 Through Hole .096 .131 .171 .216 .265 .329 .428 .531 .630 .725 Rosette C a¯ b¯

Blind Hole Hole Diameter, D0 /D Hole Diameter, D0 /D

Depth/D 0.40 0.45 0.50 0.55 0.60 0.40 0.45 0.50 0.55 0.60 0.00 .000 .000 .000 .000 .000 .000 .000 .000 .000 .000 0.06 .081 .106 .132 .163 .200 .132 .167 .199 .235 .279 0.12 .178 .230 .286 .349 .427 .309 .386 .451 .533 .624 0.18 .252 .321 .395 .475 .565 .464 .569 .666 .760 .857 0.24 .297 .375 .458 .546 .640 .576 .696 .805 .905 .997 0.30 .321 .404 .491 .583 .679 .650 .778 .893 .994 1.081 0.36 .333 .417 .507 .601 .701 .697 .829 .946 1.048 1.131 0.42 .337 .422 .514 .610 .712 .727 .860 .980 1.082 1.162 0.48 .338 .423 .516 .614 .717 .746 .881 1.001 1.103 1.182 Through Hole .316 .399 .494 .597 .707 .623 .723 .799 .847 .859

TABLE 4 Placement of the Principal Angleb

Q > 0 Q = 0 Q < 0 T < 0 45° <b < 90° 45° 0° <b < 45° T = 0 90° undeﬁned 0° T > 0 -90° < b < –45° –45° –45° < b < 0°

of s_{max}will closely correspond to the direction of the
numeri-cally most negative (compressive) relieved strain.

NOTE 8—The clockwise (CW) measurement direction for angleb

deﬁned in 9.1.10 applies only to a strain gage rosette with CW gage numbering, such as that illustrated in Fig. 2. The opposite measurement direction forbapplies to a counter-clockwise (CCW) strain gage rosette. In such a rosette, the geometrical locations of gages 1 and 3 are interchanged relative to the CW case. The new gage 1 becomes the reference gage. For a CCW rosette, a positive value of b, sayb= 30°, indicates thatsmaxlies 30° counter-clockwise of the direction of gage 1.

All other aspects of the residual stress calculation are identical for both CW and CCW rosettes.

9.1.10 If either of the computed principal stresses exceeds 60 % of the material yield stress, then some localized yielding has occurred in the material around the hole. In this case, the results are not quantitative, and must be reported as “indica-tive” only. In general, the computed stresses whose values exceed 60 % of the material yield stress tend to be overesti-mated. Their actual values are usually smaller than indicated.

9.2 “Thick” Workpiece:

9.2.1 Plot graphs of strains e_{1}, e_{2},e_{3} versus hole depth and
conﬁrm that the data follow generally smooth trends.
Investi-gate substantial irregularities and obvious outliers. If necessary,
repeat the hole-drilling test.

9.2.2 For each set of e_{1},e_{2}, e_{3} measurements, calculate the
corresponding combination strains p, q and t using Eq 3-5.

9.2.3 Verify that the residual stresses are uniform within the hole depth. Identify the set of combination strains q or t that contains larger absolute values. Express each set of combina-tion strains p and the larger of q and t as a percentage of their values at the maximum speciﬁed hole depth. Plot these percent strains versus hole depth. These graphs should yield data points very close to the curves shown in Fig. 6 (17). Data points that are signiﬁcantly separated from the curves in Fig. 6, say by more than 63 %, indicate either substantial stress non-uniformity through the material thickness, or strain measure-ment errors. In either case, the measured data are not accept-able for uniform residual stress calculations. Further measurements for non-uniform residual stresses may be appro-priate, see 8.5.

NOTE 9—This graphical test is not a sensitive indicator of stress ﬁeld

uniformity. Workpieces with signiﬁcantly non-uniform stress ﬁelds can yield percentage relieved strain curves substantially similar to those shown in Fig. 6. The main purpose of the test is to identify grossly non-uniform stress ﬁelds and strain measurement errors. This stress uniformity test is available only when working with “thick” workpieces.

9.2.4 For each of the hole depths corresponding to the eight
sets of e_{1}, e_{2}, e_{3} measurements, use Table 3 to determine the
numerical values of the calibration constants a– and b–
corre-sponding to the hole depth and diameter, and the type of rosette
used. The numerical values in this table derive from ﬁnite
element analyses (4).

9.2.5 Compute the three combination stresses P, Q and T corresponding to the three sets of combination strains p, q, and t using the following formulas (18):

P5 –_{1} E _{1 n}

### (

~a·p!### (

~a2! (14) Q 5 –E### (

~b·q!### (

~b2! (15) T 5 –E### (

~b·t !### (

~b2! (16)where S indicates a summation of the indicated quantities for the eight hole depths.

NOTE 10—It is possible to evaluate the combination stressesP,Qand

T using Eq 3-8 with only one set of the e1, e2, e3 measurements, for

example, the values at the maximum hole depth. Such a calculation could be useful to give a quick residual stress estimate. However, the averaging method used in 9.2.5 is preferred because it uses all the measured strain data, and it signiﬁcantly reduces the effects of random strain measurement errors (19).

9.2.6 Compute the Cartesian stresses s_{x}, s_{y} and t_{xy}, the
principal stresses s_{max} and s_{min}, and the principal angle b as
described in 9.1.5 to 9.1.10.

9.3 Intermediate Thickness Workpieces:

FIG. 6 Typical Plots of Percent of Strain versus Depth for Uniform Through-Thickness Stress, (a) Rosette Types A & B, (b)

9.3.1 The intermediate case of a workpiece whose thickness lies between the speciﬁcations for “thin” and “thick” work-pieces is outside the scope of this test method. For workwork-pieces with uniform stress, an approximate result can be obtained for such workpieces by using a through hole and interpolating the “Blind Hole” and “Through-the-thickness Hole” calibration data given in Table 3. Residual stress results obtained in this way should be reported as “nonstandard” and “approximate.” 10. Computation of Non-Uniform Stresses

10.1 Strain Data:

10.1.1 Plot graphs of strainse_{1},e_{2},e_{3}versus hole depth and
conﬁrm that the data follow generally smooth trends.
Investi-gate substantial irregularities and obvious outliers. If necessary,
repeat the hole-drilling test.

10.1.2 Compute the following combination strain vectors
for each set of measured strains, e_{1}, e_{2}, e_{3}:

p_{ j}5~e31 e1! j/2 (17)

q_{ j}5~e3–e1! j/2 (18)

t _{ j}5~e_{3}1 e_{1}– 2e_{2}!_{ j}/ 2 (19)

where the subscript j refers to the serial numbers of the hole
depth steps corresponding to the successive sets of measured
strains e_{1}, e_{2}, e_{3}.

10.1.3 Estimate the standard errors in the combination
strains (20):
p_{std }25

### (

j51 n23_{~}

_{ p}j– 3 p j1113 p j12–p j13! 2 20~n– 3! (20) q

_{std }25

### (

j51 n23_{~}

_{q}j– 3q j1113q j12–p j13! 2 20~n– 3! (21) t

_{std }25

_{(}

j51
n23 _{~}

_{t }j– 3t j1113t j12–t j13! 2 20~n– 3! (22)

where n = the number of sets of strain data at the various hole depth steps. The summation is carried out over the range 1 # j # n – 3.

10.2 Calibration Matrices:

10.2.1 If using a type A rosette, use the calibration data given in Table 5 to form the matrices a– jk and b

–

jk . The tabulated

numbers refer to a 1_{ ⁄ }_{16} _{in. nominal size rosette, which is the}

most commonly used size. If using a 1_{ ⁄ }_{32}_{in. rosette, multiply all}

hole and stress depths in the table by 0.5. If using a 1_{ ⁄ }_{8} _{in.}

rosette, multiply all hole and stress depths by 2.

10.2.2 If using a type B rosette, use the calibration data given in Table 6 to form the matrices a– jk and b

–

jk . If using a type

C rosette, use Table 7 instead. Types B and C rosettes are
generally available only in 1_{ ⁄ }_{16} _{in. nominal size.}

10.2.3 The tabulated numbers in Tables 5-7 correspond to a hole diameter of 0.080 in. (2 mm). Adjust the numbers to conform to the measured hole diameter by multiplying them by

(measured hole diameter/0.080 in.)2 or (measured hole

diameter/2 mm)2 as appropriate.

NOTE 11—The small discrepancies between the quoted inch and

millimeter dimensions are not signiﬁcant, and may be ignored.

NOTE 12—The numbers in Tables 5-7 are listed with ﬁve decimal

places to reduce round-off errors when doing calculations using an entire matrix of numbers. This format exceeds the expected precision of any individual number.

10.3 Stress Calculation Method :

10.3.1 Using the Integral Method (4), the residual stresses
within each hole depth step can be computed from the
corresponding measured strains by solving the matrix
equa-tions:4
a P 5_{1} E _{1 n}p (23)
b Q5E q (24)
b T5E t (25)
in which:
P_{k }5~~s y!k 1~s x !k ! / 2 (26)
Q_{k }5~~s y!k 1~s x !k ! / 2 (27)
T _{k }5~t_{ xy}!_{k } (28)

and where the combination strains p, q and t are as deﬁned in Eq 17-19. Stress calculations using Eq 23-25 are effective when few hole depth steps are used (4). However, for the large number of hole depth depths used here, the matrices a and b

become numerically ill-conditioned. Under these conditions, small errors in the measured strains cause proportionally larger errors in the calculated stresses. To reduce this effect, use Tikhonov regularization (20-22) as described in the following paragraphs.

10.3.2 Form the tri-diagonal “second derivative” matrix c:

(29)

where the number of rows equals the number of hole depth steps used. The ﬁrst and last rows contain zeros; all other rows have [–1 2 –1] centered along the diagonal.

10.3.3 Augment Eq 23-25 using matrix c to implement Tikhonov second-derivative (smooth model) regularization:

~aT_{a}_{1 a}
PcTc! P5
E
11 naTp (30)
~bT_{b}_{1 a}
QcTc! Q5E bTq (31)
~bTb1 a_{T }cTc! T5E bTt (32)

10.3.4 The factors a_{P}, a_{Q} and a_{T} control the amount of
regularization that is used. Regularization has the effect of
smoothing the stress results. Zero values for the factors make
Eq 30-32 equivalent to the unregularized Eq 23-25. Positive
values of the factors give regularization (smoothing) amounts
that increase as larger factors are chosen. Insufficient
regular-ization leaves excessive noise in the calculated stress results,
while excessive regularization distorts the stress results.
Opti-mal regularization balances these two tendencies.

10.3.5 Make initial guesses for the required values a_{P}, a_{Q}

anda_{T}. Small numbers in the range 10-4 to 10-6are suitable.
Solve Eq 30-32 to determine the stresses P, Q and T.

4_{Boldface type in equations indicates matrix and vector quantities. Thus a¯}

represents the set of quantities a–

TABLE 5

Table 5(a) Hole-Drilling Calibration Matrix a¯ for a1_{ ⁄ }_{16}_{in. Type A Rosette with a 0.080 in. (2 mm) Hole}A

Stress Depth

Hole Depth 0.002 0.004 0.006 0.008 0.010 0.012 0.014 0.016 0.018 0.020 in. in. mm 0.05 0.10 0.15 0.20 0.25 0.30 0.35 0.40 0.45 0.50 mm 0.002 0.05 -0.00679 0.004 0.10 -0.00815 -0.00714 0.006 0.15 -0.00937 -0.00844 -0.00734 0.008 0.20 -0.01046 -0.00960 -0.00858 -0.00739 0.010 0.25 -0.01141 -0.01063 -0.00968 -0.00856 -0.00728 0.012 0.30 -0.01223 -0.01152 -0.01064 -0.00960 -0.00839 -0.00701 0.014 0.35 -0.01291 -0.01227 -0.01147 -0.01050 -0.00936 -0.00806 -0.00659 0.016 0.40 -0.01360 -0.01287 -0.01207 -0.01132 -0.01015 -0.00893 -0.00759 -0.00615 0.018 0.45 -0.01416 -0.01344 -0.01264 -0.01184 -0.01082 -0.00970 -0.00846 -0.00712 -0.00567 0.020 0.50 -0.01463 -0.01392 -0.01312 -0.01223 -0.01134 -0.01031 -0.00917 -0.00793 -0.00657 -0.00511 0.022 0.55 -0.01508 -0.01434 -0.01354 -0.01270 -0.01173 -0.01072 -0.00977 -0.00854 -0.00730 -0.00600 0.024 0.60 -0.01545 -0.01471 -0.01391 -0.01306 -0.01211 -0.01113 -0.01013 -0.00906 -0.00791 -0.00670 0.026 0.65 -0.01578 -0.01503 -0.01422 -0.01340 -0.01243 -0.01146 -0.01049 -0.00938 -0.00842 -0.00722 0.028 0.70 -0.01606 -0.01531 -0.01450 -0.01366 -0.01271 -0.01175 -0.01078 -0.00970 -0.00869 -0.00765 0.030 0.75 -0.01629 -0.01554 -0.01473 -0.01390 -0.01294 -0.01199 -0.01102 -0.00996 -0.00892 -0.00795 0.032 0.80 -0.01649 -0.01574 -0.01493 -0.01410 -0.01313 -0.01217 -0.01123 -0.01018 -0.00919 -0.00815 0.034 0.85 -0.01665 -0.01590 -0.01510 -0.01426 -0.01330 -0.01234 -0.01138 -0.01036 -0.00938 -0.00836 0.036 0.90 -0.01679 -0.01604 -0.01523 -0.01441 -0.01344 -0.01248 -0.01151 -0.01049 -0.00955 -0.00852 0.038 0.95 -0.01692 -0.01617 -0.01536 -0.01452 -0.01357 -0.01261 -0.01164 -0.01063 -0.00967 -0.00866 0.040 1.00 -0.01704 -0.01628 -0.01548 -0.01465 -0.01368 -0.01272 -0.01176 -0.01074 -0.00978 -0.00877 Stress Depth

Hole Depth 0.022 0.024 0.026 0.028 0.030 0.032 0.034 0.036 0.038 0.040 in.
in. mm 0.55 0.60 0.65 0.70 0.75 0.80 0.85 0.90 0.95 1.00 mm
0.022 0.55 -0.00464
0.024 0.60 -0.00543 -0.00411
0.026 0.65 -0.00604 -0.00485 -0.00364
0.028 0.70 -0.00655 -0.00544 -0.00431 -0.00316
0.030 0.75 -0.00693 -0.00589 -0.00484 -0.00378 -0.00270
0.032 0.80 -0.00716 -0.00624 -0.00524 -0.00425 -0.00328 -0.00231
0.034 0.85 -0.00738 -0.00644 -0.00555 -0.00464 -0.00373 -0.00283 -0.00195
0.036 0.90 -0.00755 -0.00665 -0.00574 -0.00492 -0.00406 -0.00323 -0.00241 -0.00162
0.038 0.95 -0.00770 -0.00679 -0.00592 -0.00508 -0.00432 -0.00353 -0.00277 -0.00203 -0.00131
0.040 1.00 -0.00781 -0.00690 -0.00605 -0.00521 -0.00448 -0.00374 -0.00303 -0.00234 -0.00167 -0.00103
Table 5(b) Hole-Drilling Calibration Matrix b¯ for a 1_{ ⁄ }_{16}_{in. Type A Rosette with a 0.080 in. (2 mm) Hole}A

Stress Depth

Hole Depth 0.002 0.004 0.006 0.008 0.010 0.012 0.014 0.016 0.018 0.020 in. in. mm 0.05 0.10 0.15 0.20 0.25 0.30 0.35 0.40 0.45 0.50 mm 0.002 0.05 -0.01264 0.004 0.10 -0.01470 -0.01352 0.006 0.15 -0.01656 -0.01554 -0.01414 0.008 0.20 -0.01821 -0.01735 -0.01611 -0.01449 0.010 0.25 -0.01967 -0.01897 -0.01789 -0.01642 -0.01458 0.012 0.30 -0.02092 -0.02038 -0.01946 -0.01815 -0.01647 -0.01439 0.014 0.35 -0.02197 -0.02159 -0.02083 -0.01968 -0.01815 -0.01624 -0.01395 0.016 0.40 -0.02308 -0.02256 -0.02182 -0.02112 -0.01952 -0.01778 -0.01576 -0.01348 0.018 0.45 -0.02400 -0.02351 -0.02280 -0.02202 -0.02072 -0.01917 -0.01735 -0.01525 -0.01289 0.020 0.50 -0.02481 -0.02434 -0.02366 -0.02273 -0.02167 -0.02031 -0.01868 -0.01678 -0.01460 -0.01216 0.022 0.55 -0.02554 -0.02507 -0.02440 -0.02362 -0.02235 -0.02103 -0.01981 -0.01793 -0.01599 -0.01386 0.024 0.60 -0.02616 -0.02571 -0.02505 -0.02428 -0.02305 -0.02177 -0.02045 -0.01890 -0.01715 -0.01522 0.026 0.65 -0.02668 -0.02625 -0.02561 -0.02487 -0.02364 -0.02239 -0.02109 -0.01949 -0.01813 -0.01623 0.028 0.70 -0.02715 -0.02673 -0.02611 -0.02536 -0.02417 -0.02294 -0.02164 -0.02012 -0.01866 -0.01708 0.030 0.75 -0.02753 -0.02713 -0.02653 -0.02582 -0.02463 -0.02341 -0.02213 -0.02064 -0.01911 -0.01767 0.032 0.80 -0.02789 -0.02749 -0.02690 -0.02620 -0.02502 -0.02382 -0.02256 -0.02108 -0.01968 -0.01807 0.034 0.85 -0.02821 -0.02781 -0.02722 -0.02652 -0.02536 -0.02417 -0.02292 -0.02146 -0.02007 -0.01850 0.036 0.90 -0.02848 -0.02809 -0.02750 -0.02682 -0.02565 -0.02447 -0.02324 -0.02176 -0.02041 -0.01885 0.038 0.95 -0.02871 -0.02832 -0.02774 -0.02706 -0.02591 -0.02473 -0.02350 -0.02204 -0.02067 -0.01916 0.040 1.00 -0.02889 -0.02851 -0.02794 -0.02727 -0.02612 -0.02495 -0.02373 -0.02227 -0.02089 -0.01940 Stress Depth

Hole Depth 0.022 0.024 0.026 0.028 0.030 0.032 0.034 0.036 0.038 0.040 in. in. mm 0.55 0.60 0.65 0.70 0.75 0.80 0.85 0.90 0.95 1.00 mm 0.022 0.55 -0.01156 0.024 0.60 -0.01310 -0.01081 0.026 0.65 -0.01430 -0.01226 -0.01013 0.028 0.70 -0.01531 -0.01345 -0.01149 -0.00944 0.030 0.75 -0.01608 -0.01439 -0.01260 -0.01073 -0.00875

10.3.6 Because of the regularization used, the unregularized
strains that correspond to the calculated stresses P, Q and T
through Eq 23-25 do not exactly correspond to the actual
strains p, q and t. The “misﬁt” vectors indicate the strain
differences:
pmisfit 5p –
11 n
E a P (33)
q_{misfit }5q –_{ E }1b Q (34)
tmisfit 5t –
1
E b T (35)

10.3.7 Calculate the mean squares of the misﬁt vectors:

p_{rms}251_{n}

### (

j51 n ~ p_{misfit }!

_{ j}2

_{(36)}q

_{rms}251

_{n}

### (

j51 n ~q_{misfit }!

_{ j}2

_{(37)}t

_{rms}251

_{n}

### (

j51 n ~t_{misfit }!

_{ j}2

_{(38)}

10.3.8 If the values of p_{rms}2, q_{rms}2 and t_{rms}2 are within 5 %
of the values of p_{std}2, q_{std}2 and t_{std}2 in Eq 20-22, accept the
calculated values of P, Q and T. If not, make new guesses of
the regularization factors:

~aP!new5
p_{std }2
prms2
~aP!old (39)
~a_{Q}!_{new}5 qstd
2
q_{rms}2~aQ!old (40)
~aT !new5
t _{std }2
t _{rms}2~aT !old (41)

10.3.9 Recalculate Eq 30-41 until the 5 % criterion is obeyed. Then accept the ﬁnal values of P, Q and T.

10.3.10 Compute the Cartesian stresses:

~s x ! j5P j–Q j (42)

~s_{ y}!_{ j}5P_{ j}1Q_{ j} (43)
~t xy! j5T j (44)

10.3.11 Compute the principal stresses and direction:

~smax !k ,~smin!k 5Pk 6

### =

Qk 21T k 2 (45) bk 5 1 2arctan## S

–T_{k }–Q

_{k }

## D

(46)10.3.12 Place the angleb in the correct quadrant using the two-argument arctan function (function atan2 in some com-puter languages). Alternatively, the result from the one-argument calculation can be adjusted by 690° as necessary to place b within the appropriate range deﬁned in Table 4.

10.3.13 A positive value of b, say b = 30°, indicates that

s_{max}lies 30° clockwise of the direction of gage 1. A negative

value of b, say b = –30°, indicates that s_{max} lies 30°
counter-clockwise of the direction of gage 1.

10.3.14 In general, the direction of s_{max} will closely
coin-cide with the direction of the numerically most negative
(compressive) relieved strain. The case where both Q = 0 and
T = 0 corresponds to an isotropic stress ﬁeld, for which the

angleb has no meaning.

10.3.15 Plot graphs of s_{max} and s_{min} versus hole depth. If
several computed stresses signiﬁcantly exceed 60 % of the
material yield stress, then the results are not quantitative, and
must be reported as “indicative” only. In general, the computed
stresses whose values exceed 60 % of the material yield stress
tend to be overestimated. Their actual values are usually
smaller than indicated.

11. Report

11.1 Test Description:

11.1.1 Description of the test workpiece, 11.1.2 Material,

11.1.3 Pertinent mechanical properties, 11.1.4 Location of strain gage rosettes, 11.1.5 Model and type of rosettes used, 11.1.6 Rosette geometry, and

11.1.7 The method used to drill the hole. 11.2 “Thin” Workpiece with Uniform Stress: 11.2.1 Strain readings for each rosette, and

11.2.2 Calculated xy- and principal stresses at each rosette. 11.3 “Thick” Workpiece with Uniform Stress:

11.3.1 Plot of strain versus depth for each rosette,

11.3.2 Tabulation of strains e_{1}, e_{2}, and e_{3} for each rosette,
and

11.3.3 Calculated xy- and principal stresses at each rosette. 11.4 “Thick” Workpiece with Non-Uniform Stress:

11.4.1 Plot of strain versus depth for each rosette,

11.4.2 Tabulation of strains e_{1}, e_{2}, and e_{3} for each rosette,
11.4.3 Estimate of standard strain errors for each rosette,
11.4.4 Tabulation and plot of calculated xy-stresses versus
depth at each rosette, and

11.4.5 Tabulation of principal stresses and principal direc-tions at each rosette.

12. Precision and Bias

12.1 Experimental Technique:

12.1.1 Operator skill and expertise are probably among the most important factors on the precision of the result. Refer-ences (10) and (11) provide substantial practical guidance about how to make high-quality hole-drilling residual stress measurements. These publications are excellent preparatory reading, particularly for practitioners who infrequently make hole-drilling measurements. TABLE 5 Continued 0.032 0.80 -0.01652 -0.01511 -0.01344 -0.01172 -0.00995 -0.00812 0.034 0.85 -0.01698 -0.01549 -0.01408 -0.01251 -0.01089 -0.00921 -0.00747 0.036 0.90 -0.01736 -0.01590 -0.01441 -0.01312 -0.011591 -0.01004 -0.00847 -0.00688 0.038 0.95 -0.01769 -0.01624 -0.01480 -0.01340 -0.01213 -0.01072 -0.00928 -0.00781 -0.00632 0.040 1.00 -0.01796 -0.01655 -0.01511 -0.01367 -0.01249 -0.01121 -0.00989 -0.00856 -0.00719 -0.00581

TABLE 6

Table 6(a) Hole-Drilling Calibration Matrix a¯ for a1_{ ⁄ }_{16}_{in. Type B Rosette with a 0.080 in. (2 mm) Hole}

Stress Depth

Hole Depth 0.002 0.004 0.006 0.008 0.010 0.012 0.014 0.016 0.018 0.020 in. in. mm 0.05 0.10 0.15 0.20 0.25 0.30 0.35 0.40 0.45 0.50 mm 0.002 0.05 -0.00726 0.004 0.10 -0.00878 -0.00766 0.006 0.15 -0.01013 -0.00909 -0.00788 0.008 0.20 -0.01133 -0.01037 -0.00924 -0.00793 0.010 0.25 -0.01237 -0.01149 -0.01043 -0.00921 -0.00781 0.012 0.30 -0.01325 -0.01245 -0.01147 -0.01033 -0.00901 -0.00751 0.014 0.35 -0.01397 -0.01325 -0.01235 -0.01129 -0.01004 -0.00863 -0.00704 0.016 0.40 -0.01471 -0.01388 -0.01297 -0.01214 -0.01088 -0.00956 -0.00811 -0.00654 0.018 0.45 -0.01533 -0.01450 -0.01360 -0.01268 -0.01161 -0.01039 -0.00904 -0.00758 -0.00599 0.020 0.50 -0.01587 -0.01504 -0.01414 -0.01313 -0.01217 -0.01105 -0.00981 -0.00845 -0.00696 -0.00536 0.022 0.55 -0.01634 -0.01550 -0.01460 -0.01367 -0.01257 -0.01147 -0.01046 -0.00909 -0.00774 -0.00633 0.024 0.60 -0.01672 -0.01589 -0.01500 -0.01406 -0.01299 -0.01190 -0.01082 -0.00964 -0.00839 -0.00708 0.026 0.65 -0.01705 -0.01621 -0.01532 -0.01441 -0.01332 -0.01225 -0.01118 -0.00997 -0.00892 -0.00764 0.028 0.70 -0.01735 -0.01651 -0.01561 -0.01468 -0.01362 -0.01255 -0.01148 -0.01031 -0.00921 -0.00810 0.030 0.75 -0.01759 -0.01675 -0.01586 -0.01493 -0.01387 -0.01280 -0.01174 -0.01059 -0.00945 -0.00840 0.032 0.80 -0.01781 -0.01697 -0.01607 -0.01515 -0.01408 -0.01302 -0.01196 -0.01080 -0.00974 -0.00860 0.034 0.85 -0.01799 -0.01715 -0.01625 -0.01533 -0.01426 -0.01320 -0.01213 -0.01099 -0.00992 -0.00881 0.036 0.90 -0.01814 -0.01730 -0.01640 -0.01550 -0.01441 -0.01334 -0.01229 -0.01114 -0.01008 -0.00897 0.038 0.95 -0.01829 -0.01744 -0.01654 -0.01561 -0.01454 -0.01347 -0.01242 -0.01129 -0.01021 -0.00912 0.040 1.00 -0.01843 -0.01757 -0.01666 -0.01573 -0.01465 -0.01358 -0.01253 -0.01140 -0.01035 -0.00925 Stress Depth

Hole Depth 0.022 0.024 0.026 0.028 0.030 0.032 0.034 0.036 0.038 0.040 in.
in. mm 0.55 0.60 0.65 0.70 0.75 0.80 0.85 0.90 0.95 1.00 mm
0.022 0.55 -0.00486
0.024 0.60 -0.00572 -0.00430
0.026 0.65 -0.00637 -0.00509 -0.00379
0.028 0.70 -0.00691 -0.00571 -0.00450 -0.00327
0.030 0.75 -0.00730 -0.00619 -0.00506 -0.00392 -0.00277
0.032 0.80 -0.00753 -0.00655 -0.00549 -0.00443 -0.00339 -0.00234
0.034 0.85 -0.00775 -0.00674 -0.00581 -0.00484 -0.00387 -0.00291 -0.00195
0.036 0.90 -0.00793 -0.00695 -0.00598 -0.00514 -0.00423 -0.00333 -0.00246 -0.00162
0.038 0.95 -0.00809 -0.00710 -0.00617 -0.00528 -0.00449 -0.00366 -0.00285 -0.00207 -0.00131
0.040 1.00 -0.00822 -0.00724 -0.00632 -0.00541 -0.00466 -0.00389 -0.00314 -0.00242 -0.00172 -0.00104
Table 6(b) Hole-Drilling Calibration Matrix b¯ for a 1_{ ⁄ }_{16}_{in. Type B Rosette with a 0.080 in. (2 mm) Hole}

Stress Depth

Hole Depth 0.002 0.004 0.006 0.008 0.010 0.012 0.014 0.016 0.018 0.020 in. in. mm 0.05 0.10 0.15 0.20 0.25 0.30 0.35 0.40 0.45 0.50 mm 0.002 0.05 -0.01417 0.004 0.10 -0.01653 -0.01516 0.006 0.15 -0.01866 -0.01746 -0.01585 0.008 0.20 -0.02055 -0.01953 -0.01810 -0.01624 0.010 0.25 -0.02222 -0.02138 -0.02012 -0.01844 -0.01634 0.012 0.30 -0.02365 -0.02299 -0.02190 -0.02040 -0.01848 -0.01614 0.014 0.35 -0.02485 -0.02437 -0.02346 -0.02214 -0.02039 -0.01823 -0.01564 0.016 0.40 -0.02610 -0.02547 -0.02459 -0.02375 -0.02195 -0.01997 -0.01769 -0.01510 0.018 0.45 -0.02715 -0.02656 -0.02571 -0.02479 -0.02331 -0.02154 -0.01947 -0.01709 -0.01440 0.020 0.50 -0.02806 -0.02750 -0.02670 -0.02561 -0.02440 -0.02283 -0.02097 -0.01879 -0.01631 -0.01353 0.022 0.55 -0.02888 -0.02833 -0.02755 -0.02664 -0.02517 -0.02365 -0.02225 -0.02008 -0.01787 -0.01546 0.024 0.60 -0.02958 -0.02906 -0.02830 -0.02740 -0.02598 -0.02450 -0.02298 -0.02119 -0.01919 -0.01699 0.026 0.65 -0.03019 -0.02968 -0.02894 -0.02808 -0.02666 -0.02521 -0.02370 -0.02186 -0.02030 -0.01816 0.028 0.70 -0.03072 -0.03023 -0.02950 -0.02864 -0.02727 -0.02584 -0.02435 -0.02257 -0.02089 -0.01910 0.030 0.75 -0.03116 -0.03068 -0.02998 -0.02914 -0.02778 -0.02638 -0.02491 -0.02316 -0.02139 -0.01976 0.032 0.80 -0.03158 -0.03108 -0.03038 -0.02956 -0.02822 -0.02684 -0.02539 -0.02366 -0.02202 -0.02022 0.034 0.85 -0.03192 -0.03143 -0.03073 -0.02990 -0.02859 -0.02723 -0.02580 -0.02410 -0.02247 -0.02071 0.036 0.90 -0.03221 -0.03173 -0.03104 -0.03022 -0.02891 -0.02756 -0.02616 -0.02444 -0.02287 -0.02112 0.038 0.95 -0.03247 -0.03200 -0.03131 -0.03048 -0.02919 -0.02785 -0.02645 -0.02475 -0.02317 -0.02146 0.040 1.00 -0.03268 -0.03222 -0.03154 -0.03074 -0.02944 -0.02810 -0.02671 -0.02501 -0.02342 -0.02173 Stress Depth

Hole Depth 0.022 0.024 0.026 0.028 0.030 0.032 0.034 0.036 0.038 0.040 in. in. mm 0.55 0.60 0.65 0.70 0.75 0.80 0.85 0.90 0.95 1.00 mm 0.022 0.22 -0.01285 0.024 0.24 -0.01460 -0.01202 0.026 0.26 -0.01596 -0.01367 -0.01126 0.028 0.28 -0.01710 -0.01499 -0.01278 -0.01046 0.030 0.30 -0.01795 -0.01603 -0.01401 -0.01188 -0.00964